1 , ADVANCES, IN URANIUM ORE PROCESSING AND RECOVERY FROM NON-CONVENTIONAL RESOURCES PROCEEDINGS OF A TECHNICAL COMMITTEE MEETING VIENNA, SEPTEMBER 1983 ^5$/ INTERNATIONAL ATOMIC ENERGY AGENCY, VIENNA, 1985
3 ADVANCES IN URANIUM ORE PROCESSING AND RECOVERY FROM NON-CONVENTIONAL RESOURCES
4 The following States are Members of the International Atomic Energy Agency: AFGHANISTAN ALBANIA ALGERIA ARGENTINA AUSTRALIA AUSTRIA BANGLADESH BELGIUM BOLIVIA BRAZIL BULGARIA BURMA BYELORUSSIAN SOVIET SOCIALIST REPUBLIC CAMEROON CANADA CHILE CHINA COLOMBIA COSTA RICA CUBA CYPRUS CZECHOSLOVAKIA DEMOCRATIC KAMPUCHEA DEMOCRATIC PEOPLE'S REPUBLIC OF KOREA DENMARK DOMINICAN REPUBLIC ECUADOR EGYPT EL SALVADOR ETHIOPIA FINLAND FRANCE GABON GERMAN DEMOCRATIC REPUBLIC GERMANY, FEDERAL REPUBLIC OF GHANA GREECE GUATEMALA HAITI HOLY SEE HUNGARY ICELAND INDIA INDONESIA IRAN, ISLAMIC REPUBLIC OF IRAQ IRELAND ISRAEL ITALY IVORY COAST JAMAICA JAPAN JORDAN KENYA KOREA, REPUBLIC OF KUWAIT LEBANON LIBERIA LIBYAN ARAB JAMAHIRIYA LIECHTENSTEIN LUXEMBOURG MADAGASCAR MALAYSIA MALI MAURITIUS MEXICO MONACO MONGOLIA MOROCCO NAMIBIA NETHERLANDS NEW ZEALAND NICARAGUA NIGER NIGERIA NORWAY PAKISTAN PANAMA PARAGUAY PERU PHILIPPINES POLAND PORTUGAL QATAR ROMANIA SAUDI ARABIA SENEGAL SIERRA LEONE SINGAPORE SOUTH AFRICA SPAIN SRI LANKA SUDAN SWEDEN SWITZERLAND SYRIAN ARAB REPUBLIC THAILAND TUNISIA TURKEY UGANDA UKRAINIAN SOVIET SOCIALIST REPUBLIC UNION OF SOVIET SOCIALIST REPUBLICS UNITED ARAB EMIRATES UNITED KINGDOM OF GREAT BRITAIN AND NORTHERN IRELAND UNITED REPUBLIC OF TANZANIA UNITED STATES OF AMERICA URUGUAY VENEZUELA VIET NAM YUGOSLAVIA ZAIRE ZAMBIA The Agency's Statute was approved on 23 October 1956 by the Conference on the Statute of the IAEA held at United Nations Headquarters, New York; it entered into force on 29 July The Headquarters of the Agency are situated in Vienna. Its principal objective is "to accelerate and enlarge the contribution of atomic energy to peace, health and prosperity throughout the world". IAEA, 1985 Permission to reproduce or translate the information contained in this publication may be obtained by writing to the International Atomic Energy Agency, Wagramerstrasse 5, P.O. Box 100, A-1400 Vienna, Austria. Printed by the IAEA in Austria December 1985
5 PANEL PROCEEDINGS SERIES ADVANCES IN URANIUM ORE PROCESSING AND RECOVERY FROM NON-CONVENTIONAL RESOURCES PROCEEDINGS OF A TECHNICAL COMMITTEE MEETING ON ADVANCES IN URANIUM ORE PROCESSING AND RECOVERY FROM NON-CONVENTIONAL RESOURCES ORGANIZED BY THE INTERNATIONAL ATOMIC ENERGY AGENCY AND HELD IN VIENNA, SEPTEMBER 1983 INTERNATIONAL ATOMIC ENERGY AGENCY VIENNA, 1985
6 ADVANCES IN URANIUM ORE PROCESSING AND RECOVERY FROM NON-CONVENTIONAL RESOURCES IAEA, VIENNA, 1985 STI/PUB/689 ISBN
7 FOREWORD With the development of nuclear power, uranium has become established as an important source of energy which augments and diversifies the world's energy resources. Nuclear power has reached a stage of maturity and reliability and currently accounts for about 12% of the world's total electricity generation. Although the uranium industry is at the present time constrained by oversupply and depressed prices, this situation is not expected to continue indefinitely. Installed nuclear power generating capacity continues to increase and there need be no doubt about the long-term importance of uranium ore processing. The technology of uranium extraction has also developed to an advanced state, compared with the early years of the industry in the 1940s and 1950s. Nonetheless, there continue to be further advances and refinements. These seek to improve uranium recovery, to reduce costs, to produce uranium concentrates of higher quality and to improve the nature of the tailings for their long-term disposal. At the same time, much effort is being directed to improving the economics of the recovery of uranium from phosphoric acid, which at the present time is only marginally competitive, and to develop processes for the recovery of uranium from non-conventional resources such as coal and natural waters, including seawater. These last processes, although technically feasible, will not be economically attractive for many years but are potentially important because they may allow access to vast uranium resources. The Technical Committee Meeting on Advances in Uranium Ore Processing and Recovery From Non-conventional Resources was convened by the Agency within the framework of its continuing activities on nuclear raw materials. The meeting was held in Vienna from 26 to 29 September A total of 64 participants from 29 countries took part and 27 papers were presented. The present volume includes 18 of these papers. The main topics covered by the technical sessions were: in situ and heap leaching, improvements in conventional acid and alkaline uranium ore processing, recovery of uranium from wet-process phosphoric acid and recovery of uranium from coal and from natural waters. The technical sessions concluded with three panel discussions dealing with pre-concentration and beneficiation, in situ and heap leaching, and recovery of uranium from wetprocess phosphoric acid. The substance of these panels is also reproduced in this volume. The Agency wishes to thank all the scientists and engineers who participated in the meeting, not only for the papers but also for the contributions to the discussions. Special thanks are due to the General Chairman, W.A. Gow (Canada) and to the Panel Chairmen, Z.M. Dogan (Turkey), W. Flôter (Federal Republic of Germany) and D. Naden (United Kingdom).
8 EDITORIAL NOTE The papers and discussions have been edited by the editorial staff of the International Atomic Energy Agency to the extent considered necessary for the reader's assistance. The views expressed and the general style adopted remain, however, the responsibility of the named authors or participants. In addition, the views are not necessarily those of the governments of the nominating Member States or of the nominating organizations. Where papers Imve been incorporated into these Proceedings without resetting by the Agency, this has been done with the knowledge of the authors and their government authorities, and their cooperation is gratefully acknowledged. The Proceedings have been printed by composition typing and photo-offset lithography. Within the limitations imposed by this method, every effort has been made to maintain a high editorial standard, in particular to achieve, wherever practicable, consistency of units and symbols and conformity to the standards recommended by competent international bodies. The use in these Proceedings of particular designations of countries or territories does not imply any judgement by the publisher, the IAEA, as to the legal status of such, countries or territories, of their authorities and institutions or of the delimitation of their boundaries. The mention of specific companies or of their products or brand names does not imply any endorsement or recommendation on the part of the IAEA. Authors are themselves responsible for obtaining the necessary permission to reproduce copyright material from other sources.
9 CONTENTS REVIEW PAPER Recent advances in uranium ore processing (IAEA-TC-491/1) 3 W.A. Gow RECOVERY OF URANIUM FROM ORE Performance of Caro's acid as an oxidant at the Nabarlek mill (IAEA-TC-491/2) 17 R.J. Ring, F.E. Vautier, G. Lucas, E. Fulton, D.J. Waters Discussion 39 Uranium extraction by continuous carbonate leaching in a pipe autoclave (IAEA-TC-491/3) 41 E. S&rensen, J. Jensen Discussion 51 Development and application of solvent extraction, resin ion exchange (RIP) and liquid membrane processes for uranium recovery (IAEA-TC-491/4) 53 D. Naden, G.A. Rowden, D.J. Lunt, D. Wilson Discussion 71 Utilisation des colonnes puisées dans le traitement industriel des minerais d'uranium (IAEA-TC-491/5) 73 M. Desson, J.P. Jouin, P. Michel, C. Duchamp, E. Henry Discussion 82 Appareil automatique de dosage en ligne de l'uranium dans les usines de concentration (IAEA-TC-491/6) 83 P. Guazzoni Discussion 98 Modular plants for small deposits (IAEA-TC-491/7) 99 J.M. Josa, A. Moral, J.L. Otero, E. Sudrez Discussion 115 The acid pressure leaching process for the Key Lake Project, Canada (IAEA-TC-491/8) 117 W. Flô ter Discussion 130
10 L'Usine de Lodève. Un procède alcalin complexe pour un minerai d'uranium complexe (IAEA-TC-491/9) 131 R. Bodu, J.-P. Hébert, P. Lafforgue, G. Lyaudet, P. Michel, R. Vanhelleputte Discussion 167 A techno-economic evaluation of eight process routes for the recovery of uranium from Witwatersrand leach pulps (IAEA-TC-491/10) 169 W. T. Ruhmer Discussion 192 RECOVERY OF URANIUM FROM PHOSPHORIC ACID Extraction of uranium (IV) from wet phosphoric acid with a kerosene solution of nonylphenyl phosphoric acids (IAEA-TC-491/11) 197 H. Gôrecki Discussion 212 Research on uranium recovery from phosphoric acid in Israel: Progress and prospects (IAEA-TC-491/12) 215 Z. Ketzinel, Y. Volkman, M. Hassid Discussion 228 The new Uraphos process and the mobile pilot plant (IAEA-TC-491/13) 231 U.M.J. Boin Discussion 244 The D2T process of uranium recovery from phosphoric acid: A process model (IAEA-TC-491/14) 247 P. Gasôs, A. Moral Discussion 260 RECOVERY OF URANIUM FROM COAL AND NATURAL WATERS Recovery of uranium from coal ash (IAEA-TC-491/15) 263 /. Slivnik, A. StergarSek, Z. Berlin, Z. Krempl, P. Marijanovic, V. Valkovic Discussion 273 Uranium recovery as a byproduct from radioactive coal (IAEA-TC-491/16) 275 G. Morales, P.J. Nadal, J.L. Merino, P. Gasôs Discussion 287 Mise au point et qualification d'un échangeur mineral à base de titane pour l'extraction de l'uranium des eaux naturelles (IAEA-TC-491/17) 289 D. Alexandre, P.P. Vistoli Uranium extraction from seawater (IAEA-TC-491/18) 299 /. Bitte Discussion 311
11 PANEL REPORTS Panel I: Physical beneficiation 315 Panel II: In situ and heap leaching 317 Panel III: Recovery of uranium from wet-process phosphoric acid 319 LIST OF PARTICIPANTS 321
13 REVIEW PAPER
15 IAEA-TC-491/1 RECENT ADVANCES IN URANIUM ORE PROCESSING W.A. GOW Mineral Sciences Laboratories, CANMET, Ottawa, Ontario, Canada Abstract RECENT ADVANCES IN URANIUM ORE PROCESSING. The paper reviews the major technological improvements in uranium ore processing in recent years. Semi-autogenous grinding, where applicable, has proven to be a significant innovation that has resulted in lower capital and operating costs. On the other hand, its successful application depends on careful and extensive predesign testing and on keeping mill feed variability to a minimum. Preconcentration of ores has been successful only in a few instances. Radiometric sorting is being used in the treatment of low-grade ores in South Africa and of ore from a vein-type deposit in the United States of America. Gravity concentration with Reichert Cones is being used in South Africa. There have been innovations in leaching techniques for very high-grade and very low-grade ores. Pressure leaching has been used in treating ores with a uranium content in the range of 0.5 to 2.5% and ores containing refractory uranium minerals. In situ, in place and heap leaching techniques have found favour in the treatment of very lowgrade porous or fissured ores. Uranium plants have been turning to high-capacity thickeners and horizontal belt filters in an effort to improve the efficiency of solid-liquid separation and to reduce capital and operating costs. However, high-capacity thickeners require very close control and operate at lower underflow pulp density which results in increased losses of soluble uranium. There is still controversy over the relative advantages and disadvantages of belt filters. Ion exchange and solvent extraction processes have received much attention, probably more than any other unit operation in uranium ore processing. Continuous ion exchange (CIX), in its various forms, is the most recent innovation in ion exchange technology. The column systems that have been installed in recent years are the Himsley Column, the USBM-MCIX Column and the Cloete-Streat Column with its variants, the NIMCIX Column and the Davy Power Gas System. Two other systems that have been used are the Porter IX, with adsorption in a series of tanks, and the CHEM-SEPS in which loading, elution, scrubbing and backwashing are done in separate compartments connected through sequentially operated valves. New developments in the design of mixer-settlers for solvent extraction have been directed to reducing the shear in mixers and to reduce the area required for phase separation in order to reduce the size of the plant and the solvent inventory. Regarding precipitation, there has been a move from the use of ammonia and nitrates to strong sulphuric acid elution and stripping to reduce environmental problems. The technology for recovering uranium from wet-process phosphoric acid and from copper heap-leaching solutions continues to be improved. Research is also being done on the recovery of uranium from seawater and from coal, although suitable technology may not be available for several decades. 3
16 4 GOW 1. INTRODUCTION Current practices for extracting uranium from ores are well documented, particularly in the OECD publication Uranium Extraction Technology . To those of us in the mineral processing business it comes as no surprise to learn from this document that process selection and development for the treatment of uranium-bearing ores have been based on the uranium content, the mineralogical composition  and occurrence of the feed material, and the current state-of-the-art. These considerations are paramount for every step of the process and affect the chemistry involved, the specific technology applied, the equipment selection and the standards for economic evaluation. The choices between autogenous and conventional comminution, acid and alkaline leaching, solvent extraction and ion exchange are all dictated by the mineralogical and pétrographie occurrence. Lower recoveries may be tolerated from low-grade ore than from high-grade ore and consequently attention will be directed to less efficient operations such as heap leaching. Where values other than uranium are present, the mineralogical composition and occurrence will be a factor in dictating the sequence in which the values are recovered. The purpose of this paper is to serve as an introduction to the more detailed papers to follow on the general theme of advanced technologies in uranium ore processing, and recovery from non-conventional sources. In view of the above remarks, it is apparent that a problem arises as to the definition of an 'unconventional source'. Because of the variety of ways in which uranium occurs in nature, who is to draw the line between a 'conventional' and an 'unconventional'source? To that Canadian processor, the high-grade deposits recently discovered in Saskatchewan containing 2-3% uranium along with nickel sulphide and arsenide minerals are unconventional when compared with the low-grade conglomerates of Elliot Lake with which we Canadians have been familiar for 25 years. This is but one of many examples that could be cited. Consequently, faced with this dilemma, it was decided to describe briefly the known sources to uranium, relate those sources to the processing strategies applied to them and then leave it to the reader to differentiate between the familiar and the mysterious. 2. URANIUM OCCURRENCE Data published jointly in 1980 by the OECD and the IAEA  reported the world's reasonably assured resources of uranium, recoverable at US $ 130/kg U, to be tonnes of U, with another two and three quarter million tonnes estimated. The proportion of these resources in the major types of deposits identified is given in Table I. Detailed descriptions of these deposit types have been given in previous publications. In this paper only the characteristics that have major significance in today's processing state-of-the-art will be mentioned.
17 IAEA-TC-491/1 TABLE I. PROPORTION OF URANIUM RESOURCES IN THE MAJOR TYPES OF DEPOSIT Deposit type (%) Sandstone 39 Quartz-pebble Conglomerate 17 Proterozoic Unconformity Related 15 Disseminated 14 Vein 7 Other 8 Sandstone deposits contain from 0.05 to 0.3% U as uraninite, pitchblende and coffinite in unoxidized deposits, and carnotite, tyuyamunite and uranophane in oxidized ores. The uranium occurs in the grain-binding material. These deposits can contain up to 5% calcite and minor amounts of sulphides. Quartz-pebble conglomerates contain from 0.01 to 0.15% U as pitchblende, uraninite, brannerite and urarothorite. The presence of pyrite in concentrations of up to 5% is common, while gold is present in the South African deposits. Although mineralization occurs mainly in the cementing material, some values are present in the pebbles. Acid-consuming materials are not a serious problem occurring as sericite and chlorite. The Proterozoic Unconformity-Related deposits are large and rich containing up to 2.5% U 3 0 8, mainly as pitchblende and uraninite, in deposits containing up to tonnes of uranium. The uranium minerals occur both in disseminated and massive form. These deposits may also contain arsenides and sulphides of nickel and other metals as well as gold. Although these deposits have been known to contain high percentages of carbonate, this is the exception rather than the rule. Disseminated deposits are those associated with syenites, pegmatites, granites and the like. They contain from 0.05 to 0.15% U and exhibit a wide range of mineralogical characteristics. Some deposits such as the pegmatites of Canada and Namibia are easily treated by conventional acid leaching of the contained uraninite/uranothorite, while other deposits are highly refractory to economic processing methods. Vein deposits are those in which the uranium minerals fill the cavities of host rocks. Pitchblende and uraninite are the most common minerals present, occurring as massive chunks as well as disseminations in the adjacent host rock. The uranium contents of these deposits vary from 0.1 to 2.5%, while in some deposits a range of sulphides and arsenides are present.
18 6 GOW In addition to these five major types of uranium deposits, there are a number of low-grade sources that do not fit into this general scheme. These include uraniferous shales and lignites, phosphates, calcretes, porous limestone with the uranium occurring as thin carnotite coatings in the voids and limestone. These vary from less than 0.01% to as high as 0.1% U URANIUM ORE PROCESSING 3.1. Crushing and grinding Over the years since uranium was first mined the process used for comminution has moved from the classic approach of primary, secondary and possibly tertiary crushing in jaw, gyratory and cone crushers, followed by closed-circuit grinding in rod and ball mills, through a number of processing modifications aimed at reducing costs. In recent years the most interesting innovation has been the use of semi-autogenous grinding in a number of uranium processing operations . The original installations were completely autogenous in that run-of-mine ore was charged directly to a wet grinding mill with a diameter to length ratio of about 3:1. The large pieces of ore would reduce smaller pieces to the desired grind and in turn be reduced through abrasion and impact. It was soon found that the addition of 15 cm diameter steel balls to comprise about 5% of the charge improved grinding efficiency, and the operation became known as semi-autogenous grinding or SAG. Sandstone-type deposits are particularly suited to SAG because the uranium occurs only in the grain-binding material and reduction to grain size is all that is needed to liberate the uranium minerals. The conglomerate ores of Canada are also ground successfully by SAG units but because, in these ores, uranium occurs in the pebbles and breakage occurs across the matrix and pebbles, the whole ore must be ground to less than grain size. Consequently, the discharge from the SAG mill is ground further in conventional ball or pebble mill circuits. Similar SAG plus ball mill circuits are used on unconformity-related ores in Australia, and are planned for these occurrences in Canada. The use of SAG mills can result in significant savings both in operating and capital costs . The capital savings result from the elimination of one or more crushing stages while operating savings are due to less maintenance costs, and the near elimination of steel grinding media, which results in reduced oxidant and acid costs. On the other hand, the successful application of SAG depends on careful and extensive predesign testing. The operation must be planned to keep mill feed variability to a minimum and this may require a blending strategy if there is a high degree of ore variability in the deposit such as can be met in vein and unconformity-related ores. If ore variability is excessive, it will be difficult to control the load in the mill and this in turn will allow excessive impact of the steel balls against the liners, which could result
19 IAEA-TC-491/1 7 in liner failure. The testing must also determine the structural competence of the ore and thus its ability to form suitable grinding media. The screens and other sizing equipment used in SAG circuits must be designed to handle wood pulp and like substances to avoid clogging and excessive circulating loads. Generally speaking, where SAG is applicable it has proven to be a significant innovation in uranium ore processing circuits Preconcentration The possibility of rejecting a portion of a uranium-bearing ore either at coarse sizes ahead of comminution, or at finer sizes ahead of leaching has challenged the ingenuity of uranium metallurgists since the 1950s. The advantages are obvious and include enhancing the feed grade, the elimination of reagent consumers ahead of leaching, and the production of a 'clean' tailing. To meet the challenge electronic ore sorting, gravity and high-intensity magnetic methods and flotation have been investigated. Only in a few instances have they met with success. The lack of acceptance has been due to excessive uranium loss combined with insufficient weight rejection to the tailings. It should come as no surprise that the most successful preconcentration technology has been radiometric sorting, which of course is based on the ore characteristic specific to uranium. Modern sorters are capable of treating particles ranging from 20 to 160 mm by measuring the radiation and surface area of the particle, estimating its U grade and directing it to the retain or reject stream. Radiometric sorting is currently used in the treatment of low-grade feeds where the uranium is a byproduct in South Africa, and in treating a vein-type deposit in the USA where the uranium occurs in isolated concentrations and preconcentration is attractive because the mine is 150 km from the leach plant. In South African experience the sorter rejects material ranging from ppm U from feeds probably of ppm. The American operation rejects material containing 0.015% U from feeds of 0.27% U. The only other significant physical preconcentration currently in use is at the Palabora operation in South Africa where the tailings from the flotation plant are upgraded using Reichert Cones, shaking tables and magnetic separation to produce a 3.0% U concentrate from feed containing 35 ppm of U with a recovery of about 65%. The operation is feasible only because it is a byproduct to the copper operation Leaching The mineralogy of the ore probably affects the leaching step more than any other operation in uranium ore processing. The type and concentration of the uranium minerals present, along with the characteristics of the gangue minerals,
20 8 GOW dictate the conditions to be used in leaching. Consequently, whether acid or alkaline leaching is used, the leaching conditions applied are as variable as the characteristics of the ores being treated. Until recently, however, the variability from one process to another has been in detail rather than in fundamentals. Recently there has been a basic change in the thinking directed towards the processing of the very high-grade ores in the 0.5 to 2.5% range, and in the very low-grade ores of a few hundred parts per million where the major value is uranium. With high-grade ores it is necessary to think in terms of 99+% uranium extraction instead of 90-95% as is usual with ore containing % U Even with ores at the 0.5% U end of the scale, losses of over 5% are economically significant. To obtain these high leach extractions in short leach time, designers have turned to pressure leaching. The Key Lake operation in Canada is an example . In addition to its use on high-grade ores, pressure leaching has been applied in treating ores containing refractory uranium minerals, and for reducing the size and the energy requirements of the leaching plant. With very low-grade porous or fissured ores, in situ, in place and heap leaching techniques have found favour. In the USA at the start of 1981 some 11 in situ solution mining operations were producing over 2500 t U/a from porous low-grade sandstone deposits [ 1 ]. However, for a number of reasons, mostly economic, several of these operations have been discontinued. The technique involves pumping oxidized, alkaline leach liquor down to the sandstone beds no more than 150 metres below the surface. The uranium-bearing solution containing from ppm of uranium is recovered by continuous ion exchange techniques. In place and heap leaching are similar in principle. In both cases the leach solution is percolated down through beds of relatively coarse ore. On leaving the bottom of the beds, the solution is treated by ion exchange for uranium recovery. The main difference in the two processes is that the in place ore is often much coarser than the heap leached material. The notable recent example of these two approaches is the Agnew Lake mine in Canada . This mine was operated from 1978 to 1983 and was designed to treat two-thirds of the ore, a steeply dipping conglomerate containing about 0.05% U 3 0 8, by in place leaching. The remaining third was treated by heap leaching after crushing to minus 20 mm and piled 6 m high on surface. The leaching solution was a sulphuric acid-iron solution oxidized by bacterial action. The in place leaching did not perform as expected, mainly because the individual pieces of ore were too large after blasting and the dip of the ore body was flatter than forecast so that percolation of the leachant was not effective. The surface heap leaching operation performed as predicted by the test programme and resulted in 80% recovery of the contained uranium in two to three years. The current interest in the use of Caro's acid as an oxidant in the acid leaching of uranium ores is of note . It is said that Caro's acid is effective and results in reduced acid consumption and lime consumption in tailings neutralization operations. It has been used successfully in Australia but the economics in a specific case will
21 IAEA-TC-491/1 9 depend on the local cost of hydrogen peroxide. Calcine from the roasting or pyrite digested in sulphuric acid is also being used as an oxidant in several South African operations Liquid-solid separation Traditionally, liquid-solid separation in uranium operations has been accomplished using vacuum drum and disc filters, and thickeners with, in some cases, assistance from cyclones ahead of the thickener. This practice has been no different to that used in hydrometallurgical operations in general. In the recent past uranium plants have been turning to high-capacity thickeners and horizontal belt filters in an effort to improve the efficiency of liquid-solid separation and reduce operating and capital costs. The high-capacity thickeners result in a very significant reduction in capital cost for a given throughput. They also provide some operating savings in electrical and heat energy. On the other hand, the fast response time in these machines requires very close control, with automatic control being favoured . These thickeners operate at lower underflow pulp density than conventional thickeners and this results in increased soluble losses. There is still controversy as to the relative advantages and disadvantages of belt filters . These units are more complex than one might expect and should not be contemplated without a thorough study of the available experience. However, there are several belt filter operations in uranium plants about which little has been published. Problems met with are being solved and presumably it will not be long before definitive accounts of their operation will be available. Clarification of the leach liquor is necessary ahead of fixed-bed ion exchange and solvent extraction operations. Recent technology in Canada, Australia and the USA for this step generally has involved the use of downflow pressure sand filters. Gypsum precipitation has been a problem in these units but anthracite beds have been less prone to this problem than have sand beds. Usually a clarifying thickener of the high-capacity type has been installed ahead of the sand filters. This technology, although popular in recent plants, is still being evaluated  Uranium recovery and purification The operations concerned with the purification and upgrading of uraniumbearing leach liquor have always held a special fascination for uranium hydrometallurgists. Consequently, ion exchange and solvent extraction processes have been researched, developed and innovated probably more than any other steps in the uranium ore processing sequence. In a general survey it is possible to mention only the more significant newer developments that are attracting the greatest interest.